INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) A MIXED ELASTOPLASTIC=RIGID?PLASTIC MATERIAL MODEL ? J. HUETINK , A. H. VAN DEN BOOGAARD, A. D. RIETMAN, J. LOF AND T. MEINDERS Faculty of Mechanical Engineering, University of Twente; P.O. Box 217; 7500 AE Enschede; The Netherlands SUMMARY In forming process simulations, the rigid?plastic material model is widely used because of its numerically robust behaviour. The model yields accurate results, as long as the strain increments are large compared to the elastic limit strain. In cases where the strain increments are small e.g. in dead metal zones or in case of elastic spring back the model is unstable or inaccurate. In this paper a new integration algorithm is described for large strain plastic deformations. The algorithm degenerates to the Euler forward elastoplastic model for small strain increments and to the rigid?plastic model for large strain increments. The model benets from the advantages of both models: accuracy and fast convergence over a large range of strain increments. The applicability of the method to forming process simulations is demonstrated by several examples. Copyright ? 1999 John Wiley & Sons, Ltd. KEY WORDS: material model; plasticity; forming processes 1. INTRODUCTION Constitutive relations for plastic deformations are usually based on rate equations. For metal plasticity Drucker?s postulate states that the direction of plastic ow rate is perpendicular to the yield surface. The magnitude of the plastic ow is determined by a consistency relation, so that the current stress remains on the yield surface. For use in an incremental procedure, the plastic strain rate must be integrated to yield a plastic strain increment. Nowadays several algorithms are available. Many algorithms are based on some kind of elastic predictor=plastic corrector scheme like the schemes of Wilkins [1] and Rice and Tracy [2]. The direction of plastic ow can be interpolated between the directions calculated at the beginning and at the end of the increment. Ortiz and Popov [3] and Nikishkov and Atluri [4] analysed these methods for xed interpolation values. For large deformation analysis, the elastic part of the strain rate can be neglected. In that case the total strain increment equals the plastic strain increment and there is no need to determine the direction of the plastic ow. This rigid?plastic integration algorithm is very robust for large strain increments but lacks accuracy for small strain increments. This is a serious drawback, because even in simulations with large strain increments there are often areas with almost no deformation (dead zones). ? Correspondence to: J. Huetink, Faculty of Mechanical Engineering, University of Twente, P.O. Box 217, 7500 AE Enschede, The Netherlands. E-mail: j.huetink@wb.utwente.nl CCC 0029-5981/99/331421?14$17.50 Copyright ? 1999 John Wiley & Sons, Ltd. Received 1 September 1998 Revised 1 February 1999 1422 J. HUETINK ET AL . Eggert and Dawson [5] and Mori et al. [6] have tried to include some elasticity into a rigid? plastic or viscoplastic model. This is needed if after a forming process e.g. the elastic spring-back must be calculated or the residual stresses or if dead metal zones exist. In this paper a mixed elastoplastic=rigid?plastic material model is described that can be regarded as an elastoplastic model, that degenerates to the rigid?plastic model for large strain increments [7]. It inherits the good convergence and accuracy of the elastic predictor=plastic corrector schemes for small strain increments and the robustness and sucient accuracy of the rigid?plastic schemes at large strain increments. In Sections 2 and 3 the basic rigid?plastic and elastoplastic material models are recapitulated. In Section 4 the new mixed elastoplastic=rigid?plastic model is described. Finally, in Section 5 three examples are used to compare the performance of the three algorithms. 2. BASIC CONCEPTS For the sake of clarity, the description in this section only considers geometrically linear behaviour (small rotations). The algorithm however is not restricted to small strains and rotations if a proper correction is made for the rotating material [8; 9]. At the end of Section 4 the extension to nite deformations is presented. Furthermore, in this paper, a restriction is made to fully isotropic behaviour, associated plasticity and the Von Mises yield criterion. The total strain rate tensor is decomposed into an elastic and a plastic part: U? = U?e + U?p (1) Since the Von Mises yield function is independent of the hydrostatic pressure, stresses and strains are split into a deviatoric and dilatational part s = b ? 13 b : 11 = b + p1 (2) p = ? 13 b : 1 (3) and ee = Ue ? 13 Ue : 11 = Ue ? 13 V 1 Ve =U :1 e (4) (5) Since only volume preserving plasticity is considered, the superscript e can be omitted from the left-hand side of (5). The relation between stresses and strains can now be described in terms of the dilatational part and the deviatoric part: p = ?KV (6) s = 2Ge (7) e Here K is the bulk modulus and G the shear modulus. The dilatational part does not contribute to the plastic deformations. For Von Mises plasticity we can concentrate on the deviatoric part. In rate form (7) becomes s? = 2G e?e = 2G(e? ? e?p ) Copyright ? 1999 John Wiley & Sons, Ltd. (8) Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) ELASTOPLASTIC=RIGID?PLASTIC MATERIAL MODEL 1423 Here the elastic material stiness is considered to be constant, not depending on temperature or any other quantity. A yield function can be dened that separates the elastic from the plastic domain. Plastic ? deformation occurs if = 0 and ? = 0, elastic deformation occurs if �or � The yield function can never be larger than 0. The Von Mises yield function can be written as q (9) = 32 s : s ? yield where yield is the uniaxial yield stress. It is a function of the equivalent plastic strain dened by Z t q ? d and ? = 23 e?p : e?p (10) (t) = 0 For associated plasticity, the plastic deformation is perpendicular to the yield surface @ 3 ? s = e?p = ? @s 2 yield (11) Here ? is a plastic multiplier that can be determined by the consistency condition ? = 0. From ? (10) and (11) we easily derive that ? = . 3. TIME INTEGRATION The relations from the previous section are not readily applicable in a nite element analysis. In taking nite time steps, the rate formulation must be integrated to give a stress increment. The assumptions, used in dierent numerical integration algorithms are decisive for the accuracy and stability of the method. The stress at the end of a time increment must be calculated based on the total strain at the beginning and at the end of the increment. If the stresses do not match the weighed equilibrium condition a new strain increment will be calculated at a global level. The task of the time integration is only to calculate the stress for a known strain increment. For fast convergence of the global equilibrium a stiness matrix must be set up that is consistent with the integration algorithm [10]. In an elastoplastic analysis the strain decomposition (1) and the elastic stress?strain relation (8) can be written in incremental form s = 2G(e ? ep ) (12) Here ep cannot be determined without assumptions about the plastic multiplier ? and the plastic strain rate direction @=@s Z t1 @ d (13) ? ep = @s t0 Time t0 represents the start and t1 the end of a particular time increment. For large strain increments the choice of the direction of ep is bypassed by neglecting the elastic strain increment, leaving ep = e. This leads to a so-called rigid?plastic material model. Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) 1424 J. HUETINK ET AL . 3.1. The rigid?plastic model In a rigid?plastic model, also referred to as the ow formulation, the elastic deformations are totally ignored. That means that a calculated strain increment equals the plastic strain increment. The globally calculated displacements must however be constrained to a ?zero-dilatation? strain eld. This can be attained by e.g. a Lagrange multiplier method or by a penalty method. In a modied rigid?plastic model the dilatational elastic strain is included in the model. This results in a penalty-like method with a specic penalty factor, representing the elastic volume change [11]. For a Von Mises material model, the plastic strain rate e? is determined by (11). This equation can readily be inverted and integrated to give s= 2 yield; 1 e 3 (14) where yield; 1 is the yield stress at the end of the increment. The contribution of the pressure p to the stress tensor is calculated from the volumetric change (6) p1 1 = ? KU : 11 + p0 1 The total stress at the end of the increment can now be written as 2 yield; 1 2 yield; 1 I+ K ? 11 : U ? p0 1 b1 = 3 9 (15) (16) where I is the fourth-order unit tensor. When the equivalent plastic strain increment is very small it is set to a xed value, avoiding division by zero. In algorithmic terminology this is represented as := max(; ) (17) In this case, the material model degenerates to a Newtonian ow model. A consistent tangential stiness matrix is derived with the dierential form of (14) 2 1 e 2 2 e de ? yield; 1 dyield; 1 d + ds1 = yield; 1 2 3 3 () 3 After some work this yields yield; 1 s1 s1 2 yield; 1 : de I+ h? ds1 = 3 (yield; 1 )2 (18) (19) with h = (dyield )= d. With db1 = ds1 + K11 : dU and de = (I ? 13 11) : dU the consistent stiness matrix is now dened as yield; 1 s1 s1 2 yield; 1 2 yield; 1 I+ h? 11 (20) + K ? D= 3 9 (yield; 1 )2 For the rst iteration from the previous increment is used. Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) ELASTOPLASTIC=RIGID?PLASTIC MATERIAL MODEL 1425 3.2. Elastoplastic model Elastic strain increments cannot be ignored for small strains or if elastic spring-back or residual stresses must be calculated. In that case an elastoplastic model must be used. First, a trial stress is calculated based on elastic deformations. If this trial stress at the end of the increment happens to be outside the elastic domain, a plastic strain is calculated in the direction of the deviatoric stress. The magnitude is determined by the consistency condition. For the calculation of the stress increment we start o with the generalized trapezoidal rule as in Ortiz and Popov [3]. The plastic strain increment is considered to be in the direction between the normal to the yield surface at the start of the increment (at known stress s0 ) and the normal to the yield surface at the end of the increment (at yet unknown stress s1 ) s1 = s0 + 2G(e ? ep ) s0 3 t = t0 ? e?p0 = ?0 2 yield; 0 s1 3 t = t1 ? e?p1 = ?1 2 yield; 1 (21) (22) (23) The weighing of the start and the end directions is done by introducing a weighing factor . Suppose ?0 =yield;0 ? ?1 =yield; 1 then Z t1 e?p d ep = t0 = (1 ? )e?p0 t + e?p1 t = (1 ? )e0p + e1p 3 [(1 ? )s0 + s1 ] = 2 yield (24) then we have with (21): 3G 3G (1 ? ) + 2Ge ? s1 s1 = s0 1 ? yield yield (25) Ortiz and Popov studied the accuracy and stability of integration algorithms for a xed value of [3]. The choice of = 1 leads to the well-known elastic predictor, radial return method. In that case the elastic predictor calculates a deviatoric trial stress s? s? = s0 + 2Ge (26) If (s? ; )�a plastic corrector is calculated based on the direction @=@s at the location of s? . In a Von Mises material model, the direction of plastic strain will remain constant during radial return and only is variable. Equation (25) can then be rewritten as 3G s = s? (27) 1+ yield The value of is derived from the consistency relation (b; ) = 0 leading to q yield + 3G = 32 s? : s? Copyright ? 1999 John Wiley & Sons, Ltd. (28) Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) 1426 J. HUETINK ET AL . Here yield is a function of the equivalent plastic strain , therefore (28) is a scalar non-linear relation, that can be solved e.g. by a Newton?Raphson method. The hydrostatic part of the stress tensor is directly related to the dilatational strain (6) p = ? KUV The nal stress is calculated from (6) and (27) b = s ? p1 = s? + K11 : U 1 + 3G=(yield ) (29) The consistent tangential stiness matrix is derived from the dierential form of (27). After some work this yields " # 3Gss 1 2GI ? 1 ? h : de (30) ds = 2 1 + 3G=(yield ) yield (1 + h=3G)yield With b = s + K11 : U and de = (I ? 13 11) : dU the consistent stiness matrix is now dened as " # 3Gss 1 2GI ? 1 ? h D= 2 1 + 3G=(yield ) yield (1 + h=3G)yield 1 2 11 (31) + K? G 3 1 + 3G=(yield ) This relation diers from the stiness matrix based on the continuum equations. Only for = 0 both matrices are equal. 4. THE MIXED ELASTOPLASTIC=RIGID?PLASTIC MODEL For the elastoplastic model the iterative process may fail due to large strain increments. For the rigid?plastic model two situations may lead to numerical failure for small strain increments. If the lower bound value in (17) is set to a small value e.g. = 10?10 then the stress is forced to the yield surface, even if in reality the situation would be elastic. This will lead to very bad convergence and locally wrong results. This may be alleviated by setting to a value that represents the strain increment from zero stress to the yield surface. However, in this case the rigid?plastic model degenerates to a viscous model for small strain increments. Consequently the strains will be considerably overestimated in regions with (almost) rigid body motions. Convergence is usually very good in this case, but the results may be (very) wrong in large parts of the model. Basically the rigid?plastic model fails because of the inability to model elastic strains. It is the purpose of the newly introduced mixed model to combine the accuracy of the elastoplastic model and the stability of the rigid?plastic model over a large range of strain increments. The starting point of the mixed model is the elastoplastic equation (25). The value of however is not xed beforehand, but is chosen depending on the value of . Note that this approach is still a valid elastoplastic approach if the value of is bounded between 0 and 1, based on a monotonous increase from s0 to s1 as in (22) and (23). Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) ELASTOPLASTIC=RIGID?PLASTIC MATERIAL MODEL 1427 Figure 1. Two possible -functions For convenience, we introduce a reference strain increment ref (corresponding to an elastic stress increment from zero to the yield stress) ref = yield 3G (32) After substitution of (32) in (25) and bringing all terms with s1 to the left we get = s0 1 ? (1 ? ) + 2Ge s1 1 + ref ref (33) It is argued that for large strain increments, the inuence of the initial stress s0 must vanish. This leads to the condition lim (1 ? ) ?? =1 ref An appropriate choice which satises this condition is ? ?0 if 6 ref ref = ?1? if � ref (34) (35) Substituting (35) into (33), using (32), and elaborating to an explicit expression for s1 results into ( 1 ? (=ref ) s0 + 2Ge for 6ref (36) s1 = 2G=(=ref ) e = 23 yield =e for �ref Comparing (36) for �ref with (14) we see that for large strain increments this model equals the rigid?plastic model, due to the particular choice of according to (35). For small strain increments this model equals the Euler forward explicit time integration. Before algorithm (36) is used an elastic prediction is performed to nd out whether any plastic deformation happens. In case of an elastic initial situation and plastic nal situation rst the intersection point with the yield surface is calculated. The presented algorithms are based on the remaining strain increment. In Figure 1 the choice for () is presented graphically, together with another possible choice, combining the mean-normal integration ( = 0� with the rigid?plastic model. In Figure 2 the elastic trial stress s? is plotted for a strain increment of magnitude ref in the -plane. It can easily be seen by the parallelogram construction that the return mapping with the Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) 1428 J. HUETINK ET AL . Figure 2. The -plane, where 2Ge = ref Euler forward integration yields the same stress s1 as the rigid?plastic algorithm with the same strain increment. This assures that both integration methods will yield the same stress at a strain increment size where the method will switch from elastoplastic to rigid?plastic. The consistent stiness matrix for large strain increments naturally equals the consistent stiness matrix for the rigid?plastic model. Since the described algorithm is proposed for large strain increments, the algorithm must be applicable in a large deformation analysis. Objective integration is obtained by using a corotational formulation [8]. The initial deviatoric stress in (36) for 6ref is substituted by s00 s00 = Rs0 RT (37) where R follows from the polar decomposition of the incremental deformation gradient F. Equation (37) only applies if the strain increment is small (i.e. � ref ). As for commonly applied metals ref is of the order 10?3 , the deformational part of F is almost negligible. Hence R may be replaced by F without loss of accuracy and the polar decomposition can be omitted. In equation (36), for large strain increments, the initial stress s0 does not appear and no special action has to be taken to take large rotations into account. This is a well-known property of the regular (rigid?plastic) ow formulation. In some of the following examples a comparison is made between the models. The predictions obtained for the classical elastoplastic model are based on an Euler backward formulation, including the corrections for objective integration (37). 5. APPLICATIONS In this section three examples are presented. The rst example is a small tension test with nonuniform deformations, due to the boundary conditions. The convergence behaviour of the dierent methods is presented for dierent sizes of strain increments. The rigid?plastic model is used with a small lower bound = 10?10 leading to a bad convergence for small strain increments. The second example is a deep drawing simulation. This example suers from an inaccurate plastic strain calculation in the rigid?plastic analysis because of a relatively high lower bound = yield =3G = ref . In the third example the inuence of is demonstrated in a plane strain compression test. Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) ELASTOPLASTIC=RIGID?PLASTIC MATERIAL MODEL 1429 Figure 3. Number of iterations needed for dierent models 5.1. Constrained tension test In this example, a small patch of 9 plane strain elements is stretched in vertical direction. Linear displacement elements with constant dilatation [12] are applied. The material model is ideally plastic with a yield stress of 30 MPa and if applicable a Young?s modulus of 78 000 MPa and a Poisson?s ratio of 0� The total height and width of the patch are initially 100 mm. At the upper and lower boundary the displacements are suppressed in horizontal direction. Due to contraction in the central part of the patch a nonuniform deformation occurs, see Figure 3(a). The analysis was performed with dierent magnitudes of displacement increments and with the radial return, rigid?plastic and mixed elastoplastic=rigid?plastic model. The Newton?Raphson iterations were stopped at a mechanical unbalance ratio of 2 � 10?6 . For the rigid?plastic model a lower bound = 10?10 was used. One displacement increment was taken to enter the plastic regime in all models. After that 10 displacement increments were imposed. For every case the number of iterations in the last increment is presented in Figure 3(b). It can be clearly seen that for small strain increments, the elastoplastic model converges fast and the rigid?plastic model does not converge at all. This is due to the fact that in the denominator becomes very small. On the other hand for large strain increments the elastoplastic model fails and the rigid?plastic model converges fast. The mixed elastoplastic=rigid?plastic model equals the rigid?plastic model for large strain increments and shows a good convergence for small strain increments. 5.2. Deep drawing of a rectangular product Deep drawing is a deformation process in which a sheet metal, the blank, is forced to deform plastically. The specic shape of the punch and die is transferred to the sheet during the forming operation. A blank holder is used to avoid wrinkling of the blank. A principle outline of this process is given in Figure 4. The deep drawing of a specic rectangular product will be used to illustrate the behaviour of the mentioned material models, i.e. the rigid?plastic material model, the elastoplastic material model and the mixed elastoplastic=rigid?plastic material model. In the rigid?plastic model the lower bound is related to the maximum elastic deformation: = yield =3G. Simulations are performed with the implicit nite element code DIEKA. Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) 1430 J. HUETINK ET AL . Figure 4. Deep drawing scheme Figure 5. Tool geometry of the rectangular product The geometry of the tools, used for the deep drawing of a rectangular product, is given in Figure 5. The product depth is 100 mm. The used blank is 600 mm � 470 mm and has a thickness of 0�mm. The blank is meshed with 4160 three-node triangular elements based on membrane theory with 1 integration point in its plane. Contact between the sheet and the tools is described with contact elements [13], in which a friction coecient of 0� is assumed. A rst set of simulations is performed with an incremental step size of 0�mm in which the three material models are applied separately. The plastic thickness strain distributions in the rectangular product after 75 mm deep drawing are depicted in Figure 6 for the rigid?plastic material model, in Figure 7 for the elastoplastic material model and Figure 8 for the mixed elastoplastic=rigid?plastic material model. One can note that the used material model inuences the plastic thickness strain distribution drastically. The thickness reduction is the highest for the rigid?plastic material model and the lowest for the elastoplastic material model. The plastic thickness strain distribution of the mixed material model inclines towards the plastic thickness strain distribution of the elastoplastic material model. The dierence in thickness strain is most notable at the bottom of the product. As a result of the higher calculated strain in the bottom the draw-in at the right-hand side of the ange is much lower for the rigid?plastic model than for the other two models. Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) ELASTOPLASTIC=RIGID?PLASTIC MATERIAL MODEL 1431 Figure 6. Plastic thickness strain distribution, using the rigid?plastic material model Figure 7. Plastic thickness strain distribution, using the elastoplastic material model The convergence behaviour of the simulations diers signicantly as well. The mechanical unbalance ratio is set at 2 per cent. The simulation with the rigid?plastic material model needs 1 iteration per incremental step for convergence. The simulation with the elastoplastic material model needs 1 to 5 iterations per step for convergence. The simulation with the mixed material model needs 3 iterations per step for convergence. The nal product depth of 100 mm is successfully reached in the simulation with the rigid? plastic material model and the mixed material model. However, the simulation with the elastoplastic material model diverges after 93 mm deep drawing. The plastic thickness strain distribution after 100 mm deep drawing along line A?B, see Figure 5, is depicted in Figure 7 for the rigid?plastic material model and the mixed material model. In Figure 9 it can be seen clearly that the calculated plastic thickness strain in case of the rigid?plastic material model is higher than the plastic thickness strain in case of the mixed material model, especially in the bottom of the product. This can be attributed to the relatively high lower bound value of . Eectively, the rigid?plastic model reduces to a viscous model in regions where Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) 1432 J. HUETINK ET AL . Figure 8. Plastic thickness strain distribution, using the mixed elastoplastic=rigid?plastic material model Figure 9. The plastic thickness strain distribution along line A?B the strain rate is low (the bottom), leading to an overestimation of the total strain. With a lower bound of = 10?7 the accuracy should improve, but then the simulation did not converge. 5.3. Compression test The third example is the 3D simulation of a plane strain compression (PSC) test. It is commonly used to determine the material behaviour of metals because of the simple geometry and the fact that the deformation is quite similar to that of rolling. The PSC test is outlined in Figure 10. In a nite element simulation it is sucient to model only one-eighth of the specimen because of the triple symmetry. In the current example the die width w is 15 mm and the initial length l0 and height h0 of the specimen are 60 and 10 mm, respectively. 1400 linear hexahedral elements with constant dilatation and 140 3D contact elements are used. The die is modelled as a rigid tool. Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) ELASTOPLASTIC=RIGID?PLASTIC MATERIAL MODEL 1433 Figure 10. PSC test before and after deformation Figure 11. Calculated edges in top view The height reduction is 60 per cent with a die speed v of 10 mm=s. With the implicit code DIEKA simulations are performed with the elastoplastic model, the rigid?plastic model with a tiny lower bound = 10?10 and high (classic) lower bound = y =3G, respectively, and with the mixed elastoplastic=rigid?plastic model. The calculated deformations for the elastoplastic, rigid?plastic ( = 10?10 ) and mixed elastoplastic=rigid?plastic models almost coincide. Only the results of the classic rigid?plastic method deviate signicantly. The calculated mid-plane product contour for this model and the mixed model are depicted in Figure 11. From these gures one can see that the specimen in case of the rigid?plastic model with high lower bound shows deformation in the rigid region, reected by the curvature of the sides. With the mixed model the rigid region is described completely elastic and therefore no signicant deformation occurs. Indexing the CPU time of the rigid?plastic model ( = 10?10 ) 100 per cent the elastoplastic model scores 86 per cent and the mixed model 74 per cent. Comparing the CPU times of the three remaining methods one can conclude that the mixed model should be preferred to the elastoplastic and rigid?plastic models. 6. CONCLUSION A new integration method for elastoplastic material models was introduced that degenerates to the rigid?plastic model for large strain increments. The mixed elastoplastic=rigid?plastic model Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999) 1434 J. HUETINK ET AL . presents a robust way of integrating the rate equations of plasticity for a large range of strain increments. The model can be regarded as an elastoplastic model with a special time-integration scheme based on a generalized trapezoidal rule using the plastic strain rates at the beginning and the end of an increment. It appears that a particular choice of the weight factor for the contribution of the begin and end of an increment, depending on the size of the increment, yields the same results as a rigid?plastic model. Physically the weight factor should be between 0 and 1. As there are only numerical considerations for the choice of any numerical integration (Euler backward, Euler forward, mean normal) or return mapping algorithms within this range, the presented model contains no additional restrictions or assumptions with respect to the material properties that can be described. Future research will be focused on the choice of the weighing function and on the implementation of this model for orthotropic yield functions and rate-dependent plasticity. REFERENCES 1. Wilkins ML. Calculation of elastic?plastic ow. In Methods of Computational Physics, Vol. 3, Alder B. et al. (eds). Academic Press: New York, 1964; 211?263. 2. Rice JR, Tracy DM. Computational fracture mechanics. In Symposium on Numerical and Computational Methods in Structural Mechanics; Urbana; Illinois; 1971, Fenves SJ (ed.). Academic Press: New York, 1973; 585 ? 623. 3. Ortiz M, Popov EP. Accuracy and stability of integration algorithms for elasto?plastic constitutive relations International Journal for Numerical Methods in Engineering 1985; 21:1561?1576. 4. Nikishkov GP, Atluri SN. Implementation of a generalized midpoint algorithm for integration of elastoplastic constitutive relations for Von Mises? hardening material. Computers and Structures 1993; 49:1037?1044. 5. Eggert GM, Dawson PR. A viscoplastic formulation with elasticity for transient metal forming. Computer Methods in Applied Mechanics and Engineering 1988; 70:165 ?190. 6. Mori K, Wang CC, Osakada K. Inclusion of elastic deformation in rigid-plastic nite element analysis. International Journal of Mechanical Sciences 1996; 38:621? 631. 7. Huetink J, Van den Boogaard AH, Rietman AD, Lof J, Meinders T. A mixed elastoplastic=rigid?plastic material model. In Computational Mechanics; New Trends and Applications, Idelsohn SR, On?ate E, Dvorkin EN (eds). Barcelona, Proceedings of WCCM IV, Buenos Aires, 1998. 8. Healy BE, Dodds Jr. RH. A large strain plasticity model for implicit nite element analyses. Computational Mechanics 1992; 9:95 ?112. 9. Cuitin?o A, Ortiz M. A material-independent method for extending stress update algorithms from small-strain plasticity to nite plasticity with multiplicative kinematics. Engineering Computations 1986; 9:437? 451. 10. Simo JC, Taylor RL. Consistent tangent operators for rate-independent elastoplasticity. Computer Methods in Appllied Mechanics and Engineering 1985; 48:101?118. 11. Atzema EH, Huetink J. Incremental formulations of rigid?plastic and elastic?plastic constitutive equations for simulation of forming processes. In Computational Plasticity; Fundamentals and Applications, Owen DRJ, On?ate E, Hinton E (eds). Pineridge Press: Swansea, 1992; 1065 ?1076. 12. Nagtegaal JC, Parks DM, Rice JC. On numerical accurate nite element solutions in the fully plastic range. Computer Methods in Applied Mechanics and Engineering 1974; 4:153?177. 13. Huetink J, Vreede PT, van der Lugt J. The simulation of contact problems in forming processes with a mixed Euler? Lagrangian FE method. In Numerical Methods in Industrial Forming Processes, Thompson EG. et al. (eds). Balkema, 1989; 549?554. Copyright ? 1999 John Wiley & Sons, Ltd. Int. J. Numer. Meth. Engng. 46, 1421?1434 (1999)

1/--страниц